Wood species affects laboratory colonization rates
International Biodeterioration & Biodegradation 64 (2010) 305e308
Contents lists available at ScienceDirect
International Biodeterioration & Biodegradation
journal homepage: www.elsevier.com/locate/ibiod
Wood species affects laboratory colonization rates of Chlorociboria sp.
Sara C. Robinson*, Peter E. Laks
Michigan Technological University, UJ Noblet Forestry Building, 1400 Townsend Dr., Houghton, MI 49931, USA
a r t i c l e i n f o
a b s t r a c t
Received 12 January 2010
Received in revised form
4 March 2010
Accepted 23 March 2010
Available online 22 April 2010
This research attempted to determine conditions and wood species required to maximize xylindein
production from a Chlorociboria sp. under laboratory conditions for use in induced spalting. A pure culture of
a Chlorociboria species was isolated from fruiting bodies and grown on 2% malt extract agar. The colonies
reached a maximum diameter of 18 mm in four weeks, although the blue-green xylindein pigment continued
to diffuse through the culture media for at least eight months. In vermiculite jar tests, this Chlorociboria
isolate colonized Populus tremuloides more heavily than Acer saccharum or Betula alleghaniensis, and did not
colonize Tilia americana at all. Pre-inoculation of test blocks with white rot fungi did not signiﬁcantly affect
xylindein production, regardless of wood species.
Ó 2010 Elsevier Ltd. All rights reserved.
Chlorociboria spp. are green stain ascomycete fungi found
throughout North America (Dixon, 1975). They produce small, bluegreen disc-like apothecia on hardwood logs, although the fruiting
bodies can be difﬁcult to locate. Wood stained by Chlorociboria
is abundant and can be found in many hardwood stands, commonly
on wood that has already been colonized by white rot (Johnston
and Park, 2005).
Only two species of Chlorociboria occur in North America:
Chlorociboria aeruginascens (Nyl.) Kanouse and Chlorociboria aeruginosa (Oeder) Seaver. The species are primarily differentiated by
spore size, with the ascospores of C. aeruginascens ranging from 5 to
7 mm and those of C. aeruginosa ranging from 8 to 14 mm (Dixon,
1975). In the literature, differences in growth rate and pigmentation between the two species are not noted, and it appears that
the species are essentially identical in most aspects. As such, green
stained wood is often identiﬁed as being colonized by Chlorociboria
spp., and not by a speciﬁc species.
The unique blue-green pigment produced by Chlorociboria spp. is
xylindein, which has been extensively researched (Blackburn et al.,
1965; Edwards and Kale, 1965; Giles et al., 1979, 1990; Saikawa et al.
2000). Although produced within the hyphae, xylindein often
diffuses into the surrounding substrate (Berthet, 1964). This diffusion leads to a greater amount of colored wood per colonization area
* Corresponding author. Tel.: þ1 309 530 3924; fax: þ1 906 487 2915.
E-mail addresses: [email protected] (S.C. Robinson), [email protected] (P.E. Laks).
0964-8305/$ e see front matter Ó 2010 Elsevier Ltd. All rights reserved.
as compared to fungi that do not produce diffusible pigments.
Hence, the diffusion of xylindein can produce a relatively large
volume of pigmented substrate without extensive colonization by
the fungus. Despite the research by Berthet, however, this diffusion
has not been conﬁrmed by microscopy.
Little research has been conducted on laboratory growth of
either of the North American Chlorociboria species. C. aeruginascens
appears to be slightly more common than C. aeruginosa, grows
slowly on culture plates, and does not consistently produce bluegreen pigment (Fenwick, 1993; Dixon, 1975). Dixon notes that
C. aeruginascens pigment typically diffuses through culture
medium well beyond the colony diameter (1975). There is currently
no published information on the growth rate or xylindein diffusion
ability of C. aeruginosa. Although both species have been isolated
from numerous hardwood and softwood species, the decay ability,
wood species preference, and growth rate of North American
Chlorociboria spp. on wood is currently unknown.
Wood colonized by Chlorociboria sp. has been utilized for artistic
purposes since the 15th century, when it was used by intarsia artists
for inlay pieces that required blue-green tones, such as plants
and water (Blanchette et al., 1992). Sampling of stained pieces from
intarsia works found that the green-stained wood pieces were all
from the Populus species. The stained wood is still utilized today for
artistic purposes; in fact the vernacular term ‘green oak’ has evolved
due to the predominant growth of Chlorociboria sp. on oak (Quercus
spp.) in some regions (Dennis, 1956).
The green stain of Chlorociboria is a type of spalting. Spalting
is deﬁned as any coloration of wood due to fungal colonization
S.C. Robinson, P.E. Laks / International Biodeterioration & Biodegradation 64 (2010) 305e308
(Robinson et al., 2007). The three types of spalting include bleaching,
caused by the removal of lignin and other colored wood constituents;
zone lines, caused by intra- and inter-fungal antagonism; and
pigmentation, caused by a large mass of pigmented fungal hyphae
concentrated in one area and/or the diffusion of that pigment into the
surrounding wood. The Ohio DNR notes that maple (Acer spp.), birch
(Betula spp.), and beech (Fagus spp.) are the three most commonly
spalted woods, with spalted oak (Quercus spp.) rarely occurring due
to the high extractive content of the wood (Ohio DNR, 2009).
Research into controlled spalting for commercial and artistic
purposes has expanded within the past ﬁve years. Most research
has focused on zone line formation by white rot fungi, primarily
because these fungi are capable of both forming zone lines and
causing bleaching (Phillips, 1987; Robinson et al., 2007). However,
pigment fungi have the potential to produce a higher quality of
spalted wood, as most do not consume structural wood components. Recent studies have begun investigating the use of pigment
fungi for spalting applications (Robinson et al., 2009a, 2009b),
although results from these studies have not shown that fungal
pigments readily penetrate into wood.
This research attempts to expand current knowledge of North
American Chlorociboria species and investigate possible stimulatory mechanisms by which these fungi might be utilized in spalting
2. Materials and methods
Fruiting bodies of Chlorociboria sp. were obtained in September
2008 from a Populus sp. log in a mixed hardwood forest in Keweenaw
County, MI. The culture was grown on 2% malt extract agar and
maintained at room temperature (22 C). The culture was transferred
to fresh agar plates every three months to maintain active growth.
Kiln-dried wood from four tree species was chosen for inoculation: sugar maple (Acer saccharum Marsh.) (12% SG ¼ 0.66, 12% MC
density ¼ 710 kg/m3), basswood (Tilia americana L.) (12% SG ¼ 0.41,
12% MC density ¼ 430 kg/m3), paper birch (Betula alleghaniensis
Britt.) (12% SG ¼ 0.59, 12% MC density ¼ 636 kg/m3), and trembling
aspen (Populus tremuloides Michx.) (12% SG ¼ 0.45, 12% MC
density ¼ 483 kg/m3). Sugar maple and yellow birch were chosen
due to the prevalence of spalting occurring in these species
(Robinson et al., 2007; Ohio DNR, 2009). Basswood was chosen due
to its popularity among woodworkers as a low-density, easy-carving
wood, and trembling aspen was chosen due to the test culture
having been isolated from a Populus spp. wood. Although xylindein
is commonly found in oak wood, this species was not utilized in this
experiment due to its high extractive content and therefore its lack
of potential to be utilized with any other spalting fungus.
Fifteen 14 mm cubes of each wood type were oven dried at 40 C
for 24 h and weighed. Blocks were steam sterilized for 30 min and
then placed in vermiculite jars (4 4 12 cm ﬂint jars), which were
prepared as described in Robinson et al. (2009b). Jars were autoclaved for 30 min prior to block placement. The blocks were placed
in the jars so that the vermiculite just covered the surface of the
block. A strip of inoculum roughly 2 2 cm was placed on the top of
the block and then covered with an aspen feeder strip measuring
approximately 3 28 34 mm. A total of 45 jars were prepared,
and each jar contained only one block.
Fifteen blocks were utilized per wood species. Five were preinoculated with Trametes versicolor, 5 with Xylaria polymorpha,
and 5 were inoculated directly with Chlorociboria sp.
Five blocks from each wood species were pre-inoculated with
T. versicolor (L.) Lloyd SR003 and an additional ﬁve blocks from each
were pre-inoculated with X. polymorpha (Pers.) Grev. SR001.
T. versicolor was isolated from an A. saccharum log in Houghton Co.,
MI. X. polymorpha was isolated from an A. saccharum log in Baraga
Co., MI. The pre-inoculated jars were incubated for eight weeks in a
humidity and temperature-controlled room (27 C 2 C, 80% 5%
relative humidity). After incubation, the jars were autoclaved for
35 min, allowed to cool, and then reinoculated with the Chlorociboria isolate. Jars that were not pre-inoculated were inoculated
with Chlorociboria along with sterilized pre-inoculation jars. All 45
jars were then incubated for 24 weeks under the same conditions
After incubation, the blocks were removed from the jars, washed
to remove any adhering mycelium and vermiculite, dried overnight,
and then weighed to determine weight loss. After drying, the
transverse face with the most green stain was scanned at 2400 dpi
using an Epson Perfection V100 photo scanner. Blocks were then
cut in half to expose a radial face, then scanned again for internal
spalting. Spalting amounts (amount of visible pigmentation per
block) were analyzed using the procedure outlined in Robinson
et al. (2009a). All data were analyzed using a two-way analysis of
variance (ANOVA) with wood species and pre-treatment as independent variables. If differences were found, a Tukey HSD was run
to determine the location of the signiﬁcant difference. Percentage
data were transformed using arcsine square root to meet ANOVA
assumptions of error term variance and normality. All statistical
procedures were performed using SAS, version 9.2 of the SAS (2009)
system for Windows.
Growth of the Chlorociboria isolate on agar plates was slow, with
colonies never exceeding 18 mm in diameter regardless of incubation time or plate size (Fig. 1). Xylindein diffusion into the culture
media began after approximately four weeks of incubation, and
continued up to four months, with colony size not increasing after
four weeks of incubation. The cultures never completely covered
the surface of the plate, however xylindein diffused throughout an
entire 60 15 mm plate by eight months.
Of the wood species tested, the Chlorociboria isolate colonized
all but basswood (Table 1), with signiﬁcantly more colonization on
aspen than on any other wood species (a ¼ 0.05). No weight loss
occurred with any wood species. Birch was lightly colonized with
only three of the ﬁfteen blocks showing any amount of external
green stain e one from the X. polymorpha pre-treatment group
(3.5% green surface area) and two from the control group (3.5% and
7%). Of those three blocks, only the one from the pre-treatment
group had internal green stain (5%).
The sugar maple blocks as a group were colonized moderately
well by the Chlorociboria isolate. The control group and T. versicolor
pre-treatment group had almost the same amount of external green
stain (around 2.5% 4.75% SD). External green stain occurred much
more frequently in the X. polymorpha pretreated blocks, which had
an average of 6.79 4.45% surface area covered by green stain.
However, the green stain did not penetrate internally into the blocks.
The Chlorociboria isolate was most successful at colonizing
the aspen blocks (Fig. 2, Fig. 3). Blocks pretreated with T. versicolor
were most heavily stained (17.98 15.01% SD external green and
8.34 10.66% SD internal green). There was more external green
stain on the control blocks than the X. polymorpha pre-treatment
blocks, and of the two, only the control blocks exhibited any internal
green stain. None of the pre-treatment results were statistically
S.C. Robinson, P.E. Laks / International Biodeterioration & Biodegradation 64 (2010) 305e308
% of Surface Colored by Green Xylindein
Fig. 2. External and internal colonization of the Chlorociboria isolate on aspen blocks
(T.v ¼ Trametes versicolor, X.p. ¼ Xylaria polymorpha). Error bars represent one standard deviation.
to their maximum diameter of 5 mm in four weeks and failed to
The Chlorociboria isolate produced signiﬁcantly more external
green stain on aspen than on any other wood species. This result
is not surprising, as the Chlorociboria species isolated from 15th
century intarsia works were all from Populus sp. (Blanchette et al.,
1992) and the culture used in these experiments was also isolated from aspen. Noting the slow growth of our isolate, it is
possible that this fungus preferentially colonizes low-density wood
species with low extractive levels. Populus sp. have very low decay
resistance (USDA Forest Service, 1967), making them perhaps
more attractive as a colonizable substrate. Sugar maple also has
a low decay resistance, however its higher speciﬁc gravity (0.63
compared to 0.38 in aspen) may have played a role in the failure of
the Chlorociboria isolate to colonize internally.
Fig. 1. Chlorociboria isolate growth on 2% malt agar plates at (A) four weeks and
(B) four months (For interpretation of the references to color in this ﬁgure legend, the
reader is referred to the web version of this article).
Although the diameter growth of the Chlorociboria isolate was
small compared to other pigment fungi, the growth rate of this
isolate was far quicker than Fenwick’s (1993) isolates, which grew
Number of green stained blocks per treatment per wood species. Total number of
blocks tested per wood species is 15; total number of blocks tested per treatment is
5. * indicates statistically signiﬁcant differences between species at (a ¼ 0.05).
Fig. 3. External (A) and internal (B) colonization of the Chlorociboria isolate on nonpretreated aspen blocks (For interpretation of the references to color in this ﬁgure
legend, the reader is referred to the web version of this article).
S.C. Robinson, P.E. Laks / International Biodeterioration & Biodegradation 64 (2010) 305e308
It is unknown why the Chlorociboria isolate failed to colonize
basswood, and barely colonized birch. Neither of these species is
particularly decay resistant, and both have speciﬁc gravities comparable to maple and aspen, respectively (basswood SG: 0.37, yellow
birch SG: 0.62). All four of the wood species used are diffuse porous
hardwoods with similar pore sizes. In addition, aspen and basswood
have very similar chemical compositions (Petterson, 1984).
This research suggests that pre-treatment of wood by a whiterot fungus probably does not increase the colonization rates of
Chlorociboria sp. However, although not statistically signiﬁcant,
pre-treatment of sugar maple by X. polymorpha resulted in a four
percent increase in external green stain over the control amount,
and pre-treatment of aspen by T. versicolor caused an eight percent
increase. This pre-treatment effect may be due to the decay of
lignin and cellulose by white rot fungi. The removal of these two
wood components ‘opens up’ the matrix of the wood, which
may facilitate faster or additional avenues for xylindein diffusion or
mycelial colonization. The increased colonization may also be due
to changes in block moisture content after autoclaving.
No weight loss was caused by the Chlorociboria isolate regardless of wood species. Although Johnston and Park (2005) proposed
that Chlorociboria spp. may cause white rot due to its prevalence on
decayed wood, it is apparent from this research that our isolate did
not cause decay.
Based upon the results outlined above, it appears that Chlorociboria is an ideal fungus for laboratory spalting under certain
conditions. Unlike some other pigment fungi whose hyphae must
penetrate the substrate to affect a color change (Ceratocystis spp.
in particular), Chlorociboria sp. needs only to colonize the surface,
owing to the diffusion of xylindein throughout the wood substrate.
Although our Chlorociboria isolate preferentially colonized P. tremuloides, pre-treatment of test blocks with a white rot fungus and/or
autoclaving may allow standard laboratory spalting tests on sugar
maple to be conducted once the wood has been conditioned.
There is currently no other tested spalting fungus that can produce
the strong blue-green color of xylindein, and the use of this pigment
in spalting applications should provide an excellent addition to the
known spalting fungi.
The Chlorociboria isolate is a slow-growing fungus that reaches
its maximum colony diameter at four weeks. However, xylindein
appears to continuously diffuse from the hyphae after colony
growth has subsided, making deep wood colonization of this fungus
unnecessary to achieve a penetrating stain. This research suggests
Chlorociboria sp. may preferentially colonize Populus species over
other hardwoods, including others of low extractive content and
low speciﬁc gravity. Although pre-treatment of the wood species
with white rot fungi did not signiﬁcantly impact Chlorociboria
colonization, a small stimulatory effect did occur with some wood
species. Future research on Chlorociboria species should continue to
investigate the possible effects of white rot pre-treatment in the
colonization rates of Chlorociboria under laboratory conditions.
Berthet, P., 1964. Formes conidiennes de divers Discomycetes. Bulletin de Societe
Mycologique 80, 125e149.
Blackburn, G.M., Ekong, D.D., Neilson, A.H., Todd, L., 1965. Xylindein. Chimia 19,
Blanchette, R.A., Wilmering, A.M., Baumeister, M., 1992. The use of green-stained
wood caused by the fungus Chlorociboria in intarsia masterpieces from the 15th
century. Holzforschung 46 (3), 225e232.
Dennis, R.W.G., 1956. A revision of the British Helotiaceae in the herbarium of
the Royal Botanical Gardens, Kew, with notes on related European species.
Mycological Papers 62 (4), 46e47.
Dixon, J.R., 1975. Chlorosplenium and its segregates. II. The genera Chlorociboria and
Chlorencoelia. Mycotaxon 1 (3), 193e237.
Edwards, R.L., Kale, N., 1965. The structure of xylindein. Tetrahedron 21, 2095e2107.
Fenwick, G.A., 1993. Chlorociboria aeruginascens in laboratory culture. The Mycologist 7 (4), 172e175.
Giles, R.G.F., Reuben, M.K., Roos, G.H.P., 1979. A quinonoid naphthopyranone as
a model for the synthesis of the pigment xylindein. Photochemical formation of
the lactone ring. South African Journal of Chemistry 32, 127e129.
Giles, R.G.F., Green, I.R., Hugo, V.I., 1990. Model studies towards xylindein precursors. South African Journal of Chemistry 43, 28e33.
Johnston, P.R., Park, D., 2005. Chlorociboria (Fungi, Helotiales) in New Zealand. New
Zealand Journal of Botany 43, 679e719.
Ohio DNR, 2009. The spalted wood. Online at. http://www.ohiodnr.com/tabid/5255/
Petterson, R.C., 1984. The Chemical Composition of Wood. U.S. Department of
Agriculture, Forest Service, Forest Products Laboratory. Madison, WI.
Phillips, L.W. 1987. The nature of spalted wood: analysis of zone line formation
between six white rot fungi. Master of Science thesis, Brigham Young University, Provo, Utah, USA.
Robinson, S.C., Richter, D.L., Laks, P.E., 2007. Colonization of sugar maple by spalting
fungi. Forest Products Journal 57 (4), 24e32.
Robinson, S.C., Laks, P.E., Turnquist, E.J., 2009a. A method for digital color analysis of
spalted wood using Scion Image software. Materials 2 (1), 62e75.
Robinson, S.C., Richter, D.L., Laks, P.E., 2009b. Effects of substrate on laboratory
spalting of sugar maple. Holzforschung 63, 491e495.
Saikawa, Y., Watanabe, T., Hashimoto, K., Nakata, M., 2000. Absolute conﬁguration
and tautomeric structure of xylindein, a blue-green pigment of Chlorociboria
species. Phytochemistry 55, 237e240.
SAS, 2009. v. 9.2. SAS Institute Inc, Cary, NC.
United States Department of Agriculture Forest Service. 1967. Comparative Decay
Resistance of Heartwood of Native Species. U.S. Forest Service Research Note: